GS2160  ZnSSiO_{2} Substrate 
n = 2.093, t = 60 nm (60.6)a

n = 2.09, t = 61.24 nm 
GS2161  GST Substrate 
n+ ik = 3.811+ i
1.629, t = 13.47 nm (13.6) 
n+ ik = 3.798+ i
1.510, t = 14.25 nm 
GS2162  Aluminum Substrate 
n+ ik = 1.778+ i
6.348, t = 34.77 nm (38.4) 
n+ ik = 1.982+ i
6.829, t = 38.76 nm 
GS2163  ZnSSiO_{2}

n
_{
1
} = 2.1,b
t
_{
1
} = 59.44 nm (60.6) 
n
_{
1
} = 2.101, t
_{
1
} = 57.23 nm 
 GST (amorphous) 
n
_{
2
}+ ik
_{
2
} = 4.382+ i
2.107, t
_{
2
} = 11.56 nm (13.6) 
n
_{
2
}+ ik
_{
2
} = 4.091+ i
1.820, t
_{
2
} = 14.39 nm 
 ZnSSiO_{2} Substrate 
n
_{
3
} = 2.09, t
_{
3
} = 29.92 nm (30.3) 
n
_{
3
} = 2.108, t
_{
3
} = 29.72 nm 
 ZnSSiO_{2}

n
_{
1
} = 2.090, t
_{
1
} = 57.53 nm (60.6) 
n
_{
1
} = 2.103, t
_{
1
} = 59.02 nm 
 GST (crystalline) 
n
_{
2
}+ ik
_{
2
} = 4.05+ i
3.851, t
_{
2
} = 14.22 nm (13.6) 
n
_{
2
}+ ik
_{
2
} = 4.109+ i
3.772, t
_{
2
} = 14.53 nm 
 ZnSSiO_{2} Substrate 
n
_{
3
} = 2.101, t
_{
3
} = 28.56 nm (30.3) 
n
_{
3
} = 2.10, t
_{
3
} = 29.11 nm 
GS2164  Aluminum  
n
_{
1
} = 2.111, t
_{
1
} = 60.63 nm (60.6) 
 ZnSSiO_{2}
 
n
_{
2
}+ ik
_{
2
} = 4.534+ i
1.936, t
_{
2
} = 11.68 nm (13.6) 
 GST (amorphous)  
n
_{
3
} = 2.09, t
_{
3
} = 30.2 nm (30.3) 
 ZnSSiO_{2} Substrate  
n
_{
4
} + ik
_{
4
} = 2.257+ i
6.907, t
_{
4
} = 33.74 nm (38.4) 
 Aluminum  
n
_{
1
} = 2.10, t
_{
1
} = 60.51 nm (60.6) 
 ZnSSiO_{2}
 
n
_{
2
}+ ik
_{
2
} = 4.320+ i
3.946, t
_{
2
} = 11.94 nm (13.6) 
 GST (crystalline)  
n
_{
3
} = 2.093, t
_{
3
} = 30.41 nm (30.3) 
 ZnSSiO_{2} Substrate  
n
_{
4
} + ik
_{
4
} = 1.952+ i
6.926, t
_{
4
} = 35.44 nm (38.4) 
GS2165  ZnSSiO_{2}

n
_{
1
}+ ik
_{
1
} = 1.989+ i
6.820, t
_{
1
} = 38.76 nm (38.4)  
 GST (amorphous) 
n
_{
2
} = 2.092, t
_{
2
} = 34.69 nm (30.3)  
 ZnSSiO_{2}

n
_{
3
}+ ik
_{
3
} = 4.175+ i
1.901, t
_{
3
} = 13.42 nm (13.6)  
 Aluminum Substrate 
n
_{
4
} = 2.099, t
_{
4
} = 59.43 nm (60.6)  
 ZnSSiO_{2}

n
_{
1
}+ ik
_{
1
} = 1.957+ i
6.792, t
_{
1
} = 36.42 nm (38.4)  
 GST (crystalline) 
n
_{
2
} = 2.099, t
_{
2
} = 28.5 nm (30.3)  
 ZnSSiO_{2}

n
_{
3
}+ ik
_{
3
} = 3.891+ i
3.504, t
_{
3
} = 16.49 nm (13.6)  
 Aluminum Substrate 
n
_{
4
} = 2.099, t
_{
4
} = 58.71 nm (60.6)  
GS2168  Aluminum  
n
_{
1
} = 2.111, t
_{
1
} = 59.16 nm (60.6) 
 ZnSSiO_{2}
 
n
_{
2
}+ ik
_{
2
} = 4.337+ i
1.871, t
_{
2
} = 12.82 nm (13.6) 
 GST (amorphous)  
n
_{
3
} = 2.111, t
_{
3
} = 29.95 nm (30.3) 
 ZnSSiO_{2} Substrate  
n
_{
4
} + ik
_{
4
} = 1.977+ i
6.815, t
_{
4
} = 37.91 nm (38.4) 
 Aluminum  
n
_{
1
} = 2.108, t
_{
1
} = 57.6 nm (60.6) 
 ZnSSiO_{2}
 
n
_{
2
}+ ik
_{
2
} = 3.651+ i
3.320, t
_{
2
} = 17.26 nm (13.6) 
 GST (crystalline)  
n
_{
3
} = 2.089, t
_{
3
} = 29.11 nm (30.3) 
 ZnSSiO_{2} Substrate  
n
_{
4
} + ik
_{
4
} = 1.807+ i
6.843, t
_{
4
} = 28.33 nm (38.4) 
GS2169  Aluminum Substrate

n+ ik = 1.896+ i
6.264, t = 18.98 nm (18.4)

n+ ik = 1.949 + i
6.711, t = 17.32 nm (18.4)
